Ageing Effects on Microstructure, Mechanical Properties ... Ageing Effects on Microstructure,...
Embed Size (px)
Transcript of Ageing Effects on Microstructure, Mechanical Properties ... Ageing Effects on Microstructure,...
Research Article Ageing Effects on Microstructure, Mechanical Properties, and Fracture Behaviour of 9Cr-1.5Mo-1Co-VNbBN Martensitic Steel Welded Joint for High Temperature Application
Ladislav Falat,1 Viera Homolová,1 Lucia Hiripová,1 Peter Ševc,1 and Milan Svoboda2
1 Institute of Materials Research, Slovak Academy of Sciences, Watsonova 47, 04001 Košice, Slovakia 2Institute of Physics of Materials, Academy of Sciences of the Czech Republic, Žižkova 22, 61662 Brno, Czech Republic
Correspondence should be addressed to Ladislav Falat; firstname.lastname@example.org
Received 3 October 2016; Accepted 10 January 2017; Published 31 January 2017
Academic Editor: Akihiko Kimura
Copyright © 2017 Ladislav Falat et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
This paper deals with long-term ageing effects of 9Cr-1.5Mo-1Co-VNbBN (CB2) steel weldment on its impact toughness, creep rupture behaviour, and hardness in relation to microstructure and fracture characteristics. The weldment was studied in PWHT state and after isothermal expositions at 625∘C for 10000 and 30000 hours. Microstructure evolution was studied using analytical scanning and transmission electron microscopy. Charpy V-notch impact toughness tests were performed for all heat-treated states with a notch location in distinct weld regions such as weld metal (WM), heat-affected zone (HAZ), and base material (BM). The overheated HAZ region exhibited the lowest impact toughness as a result of severe welding induced microstructure degradation. Creep tests were performed at 625∘C in the stress range between 80 and 120MPa. At the highest applied stress, creep fracture occurred in WM, whereas at lower stresses the failure position shifted towards fusion zone at WM/HAZ interface. The hardness profiles experienced significant scattering due to weld microstructural heterogeneity. The major fracture mechanisms involved transgranular quasi cleavage and intergranular creep cracking in impact and creep loading conditions, respectively.
The welded joints of high chromium tempered martensitic creep-resistant steel are frequently employed in construction of modern fossil-fired thermal power plants operating at supercritical and ultrasupercritical conditions .Their main application area covers structural parts of thick section boiler components including high temperature header sec- tion and main steam pipelines [2–4]. It generally holds that local microstructure formation of individual weld regions, namely, the weld metal (WM), fusion zone (FZ), and heat- affected zone (HAZ) depends on their location within the weldment and reached peak temperature during the weld preparation. Due to the presence of microstructural gradient and welding-related residual stresses in welded joints of martensitic/ferritic power plant steel, it is necessary to per- form their postweld heat treatment (PWHT). Beside thermal stabilization of initial weld microstructure and residual stress relief, the application of PWHT decreases unallowably high
hardness in FZ and increases the weldments toughness [2, 5, 6]. Worldwide constant efforts are still being put into developments aiming for creep strength improvement of these materials. Apart from classical strengthening mecha- nisms, such as solid solution, precipitation, and subbound- ary strengthening, Abe et al.  revealed specific boron strengthening mechanism in weldments of Japanese boron alloyed 9Cr-3W-3Co-VNbBN (MARBN) martensitic steel based on the HAZ microstructure modification via boron related effects on the retardation of secondary precipitates coarsening and suppression of diffusive ferrite-to-austenite phase transformation duringwelding.TheEuropean research initiatives in the frame of international collaboration within COST Action 536 resulted in the development of a series 9Cr-Mo-Co-B-VNbBN model alloys for production of thick castings and forgings intended for the use at supercritical steam conditions . One of them is represented by 9Cr- 1.5Mo-1Co-VNbBN (CB2) steel with controlled boron and nitrogen content.
Hindawi Advances in Materials Science and Engineering Volume 2017, Article ID 6824385, 14 pages https://doi.org/10.1155/2017/6824385
2 Advances in Materials Science and Engineering
Table 1: Chemical composition in wt.% of CB2 steel BM and FM (Thermanit MTS 5 Co 1).
C Si Mn Cr Ni Mo V Ti Al Co Nb B N Fe BM 0.12 0.29 0.86 9.14 0.22 1.5 0.19 0.002 0.006 0.95 0.06 0.012 0.020 Balance FM 0.11 0.45 0.65 9.10 0.7 1.3 0.24 0.01 0.01 1.09 0.06 0.003 0.028 Balance
Our previous works [9, 10] were focused on preliminary studies of ageing effects of thick-walled CB2 weldments with respect to thermal stability of their microstructures and local mechanical properties in different loading conditions. The present study represents an extended and continuing research work aiming for deeper investigation and interpretation of the effects of long-term ageing expositions onmechanical and creep properties variations of the sameCB2 steel weldment in relation to its detailedmicrostructural and fracture character- istics.
2. Experimental Material and Procedure
The welded joint of cast 9Cr-1.5Mo-1Co-VNbBN (CB2) steel was produced by tungsten inert gas (TIG) welding using elec- trode weaving technique andmodified filler metalThermanit MTS 5 Co1 at PHB Stahlguss International. The thickness of welded plates was around 98mm. Both the base material (BM) and filler metal (FM) chemical composition is given in Table 1. After the weld preparation, subsequent postweld heat treatment (PWHT) was carried out industrially at 730∘C for 24 h by the weld producer. Cross-weld segments obtained within COST Action 536 collaboration were afterwards long- term isothermally aged at 625∘C for 10 and 30 thousand hours in our laboratory conditions. Charpy V-notch (CVN) samples with dimensions of 10 × 10 × 55mm and the notch individually located in the BM, WM, and overheated HAZ next to FZwere used to test impact toughness after long-term ageing expositions and in the PWHT state, as well. The tests were performed at room temperature (RT) for all thematerial states. After the preageing at 625∘C for 30 kh, the samples were impact tested also at 100∘C.Creep rupture tests were car- ried out at 625∘Cwith applied stresses of 80, 100, and 120MPa using round M8 tensile creep specimens with gauge length of 40mm and body diameter of 5.5mm. Cross-weld creep tests were performed for the weldments in initial PWHT state and separately also for the welds preaged at 625∘C for 30 kh. The BM preaged in the same way was also creep tested for reference. Hardness HV10 profiles were measured for as-crept material states across the welded joint samples. The microstructure of individual experimental states was observed and analyzed by means of light microscopy (LM) and scanning and transmission electron microscopy (SEM, TEM) equippedwith energy dispersiveX-ray (EDX) analyzer. Carbon extraction replicas were used for semiquantitative chemical microanalyses of metallic elements in extracted secondary phase precipitates. Experimental results of the phase analyses have been compared with those obtained by thermodynamic calculations usingThermo-Calc Classic soft- ware  and noncommercial database Steel 16 formulated by Kroupa et al. . Fractographic studies included fracture path and fracture surface observations using LM and SEM.
3. Results and Discussion
3.1. Microstructure and Phase Analysis. Overall microstruc- tural features of individual weld regions of studied CB2 weld- ment in the initial PWHT state are shown on light-optical micrographs in Figure 1. Generally, all the microstructures consist of tempered martensite with precipitated particles of secondary phases occurring within matrix as well as on all types of inner microstructural interfaces such as the primary austenitic grain boundaries, block, packet, and lath subboundaries. Apart from these common features, the microstructures of individual weld regions possess their own specific microstructural characteristics. The original cast, normalized and temperedmartensitic microstructure of BM shows noticeably coarse grains and laths (Figure 1(a)), whereas the remelted microstructure of WM (Figure 1(b)) is significantly refined due to its fast cooling during the welding. Transition region between the BM and WM is represented by notably heterogeneous HAZ microstructure following the locality of weld FZ (Figure 1(c)). Beside its heterogeneous grain size, the transition zone exhibits some minor occurrence of nonequilibrium 𝛿-ferrite grains appearing like small precipitate-free areas (see Figure 1(c)). More detailed microstructures of BM and WM in PWHT state and also in long-term aged states at 625∘C for 10 and 30 thousand hours are visualized on SEM-micrographs in Figures 2–4. In comparison to the microstructures in PWHT state (Figure 2), the microstructures after long-term ageing expositions (Figures 3 and 4) can be characterized by additional precipitation and coarsening of secondary phase particles accompanied by proceeding recovery processes of highly tempered martensitic matrix. The differences in size, morphology, and distribution of secondary precipitates occurring in PWHT state and after the 625∘C ageing for 30 kh are shown on TEM carbon extraction replicas for BM (Figure 5) and WM (Figure 6).
Phase analyses of individual precipitates on the TEM replicas were performed by their semiquantitative chemical microanalyses via local EDX measurements. The results are given in Table 2 in the form of mean